Uniaxial Mechanical Response
This chapter is intended as a review of certain fundamental aspects of mechanics of materials, using
the material’s response to unidirectional stress to provide an overview of mechanical properties
without addressing the complexities of multidirectional stress states. Most of the chapter will
restrict itself to small-strain behavior, although the last section on stress-strain curves will preview
material response to nonlinear, yield and fracture behavior as well.
1.1 Tensile Strength and Tensile Stress
Perhaps the most natural test of a material’s mechanical properties is the tension test, in which
a strip or cylinder of the material, having length L and cross-sectional area A, is anchored at one
end and subjected to an axial load P – a load acting along the specimen’s long axis – at the
other. (See Fig. 1.1). As the load is increased gradually, the axial deﬂection δ of the loaded end
will increase also. Eventually the test specimen breaks or does something else catastrophic, often
fracturing suddenly into two or more pieces. (Materials can fail mechanically in many diﬀerent
ways; for instance, recall how blackboard chalk, a piece of fresh wood, and Silly Putty break.) As
engineers, we naturally want to understand such matters as how δ is related to P, and what ultimate
fracture load we might expect in a specimen of diﬀerent size than the original one. As materials
technologists, we wish to understand how these relationships are inﬂuenced by the constitution and
microstructure of the material.
Figure 1.1: The tension test.
One of the pivotal historical developments in our understanding of material mechanical proper-
ties was the realization that the strength of a uniaxially loaded specimen is related to the magnitude
of its cross-sectional area. This notion is reasonable when one considers the strength to arise from
6 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
the number of chemical bonds connecting one cross section with the one adjacent to it as depicted in
Fig. 1.2, where each bond is visualized as a spring with a certain stiﬀness and strength. Obviously,
the number of such bonds will increase proportionally with the section’s area1. The axial strength
of a piece of blackboard chalk will therefore increase as the square of its diameter. In contrast,
increasing the length of the chalk will not make it stronger (in fact it will likely become weaker,
since the longer specimen will be statistically more likely to contain a strength-reducing ﬂaw.)
Figure 1.2: Interplanar bonds (surface density approximately 1019 m−2).
When reporting the strength of materials loaded in tension, it is customary to account for the
eﬀect of area by dividing the breaking load by the cross-sectional area:
where σf is the ultimate tensile stress, often abbreviated as UTS, Pf is the load at fracture, and A0
is the original cross-sectional area. (Some materials exhibit substantial reductions in cross-sectional
area as they are stretched, and using the original rather than ﬁnal area gives the so-call engineering
strength.) The units of stress are obviously load per unit area, N/m2 (also called Pascals, or Pa)
in the SI system and lb/in2 (or psi) in units still used commonly in the United States.
In many design problems, the loads to be applied to the structure are known at the outset, and we wish
to compute how much material will be needed to support them. As a very simple case, let’s say we wish to
use a steel rod, circular in cross-sectional shape as shown in Fig. 1.3, to support a load of 10,000 lb. What
should the rod diameter be?
Directly from Eqn. 1.1, the area A0 that will be just on the verge of fracture at a given load Pf is
All we need do is look up the value of σf for the material, and substitute it along with the value of 10,000
lb for Pf , and the problem is solved.
A number of materials properties are listed in the Materials Properties2
module, where we ﬁnd the UTS
of carbon steel to be 1200 MPa. We also note that these properties vary widely for given materials depending
on their composition and processing, so the 1200 MPa value is only a preliminary design estimate. In light
of that uncertainty, and many other potential ones, it is common to include a “factor of safety” in the
The surface density of bonds NS can be computed from the material’s density ρ, atomic weight Wa and Avogadro’s
number NA as NS = (ρNA/Wa)2/3
. Illustrating for the case of iron (Fe):
cm3 · 6.023 × 1023 atoms
= 1.9 × 1015 atoms
NS ≈ 1015 atom
cm2 is true for many materials.
1.1. TENSILE STRENGTH AND TENSILE STRESS 7
Figure 1.3: Steel rod supporting a 10,000 lb weight.
design. Selection of an appropriate factor is an often-diﬃcult choice, especially in cases where weight or cost
restrictions place a great penalty on using excess material. But in this case steel is relatively inexpensive
and we don’t have any special weight limitations, so we’ll use a conservative 50% safety factor and assume
the ultimate tensile strength is 1200/2 = 600 MPa.
We now have only to adjust the units before solving for area. Engineers must be very comfortable with
units conversions, especially given the mix of SI and older traditional units used today. Eventually, we’ll
likely be ordering steel rod using inches rather than meters, so we’ll convert the MPa to psi rather than
convert the pounds to Newtons. Also using A = πd2
/4 to compute the diameter rather than the area, we
4 × 10000(lb)
π × 600 × 106(N/m2) × 1.449 × 10−4 lb/in2
= 0.38 in
We probably wouldn’t order rod of exactly 0.38 in, as that would be an oddball size and thus too expensive.
But 3/8 (0.375 in) would likely be a standard size, and would be acceptable in light of our conservative
If the specimen is loaded by an axial force P less than the breaking load Pf , the tensile stress
is deﬁned by analogy with Eqn. 1.1 as
The tensile stress, the force per unit area acting on a plane transverse to the applied load, is a
fundamental measure of the internal forces within the material. Much of Mechanics of Materials
is concerned with elaborating this concept to include higher orders of dimensionality, working out
methods of determining the stress for various geometries and loading conditions, and predicting
what the material’s response to the stress will be.
Many engineering applications, notably aerospace vehicles, require materials that are both strong and
lightweight. One measure of this combination of properties is provided by computing how long a rod of the
material can be that when suspended from its top will break under its own weight (see Fig. 1.4). Here the
stress is not uniform along the rod: the material at the very top bears the weight of the entire rod, but that
at the bottom carries no load at all.
To compute the stress as a function of position, let y denote the distance from the bottom of the rod and
let the weight density of the material, for instance in N/m3
, be denoted by γ. (The weight density is related
to the mass density ρ [kg/m3
] by γ = ρg, where g = 9.8 m/s2
is the acceleration due to gravity.) The weight
supported by the cross-section at y is just the weight density γ times the volume of material V below y:
8 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
Figure 1.4: Circular rod suspended from the top and bearing its own weight.
W(y) = γV = γAy
The tensile stress is then given as a function of y by Eqn. 1.2 as
Note that the area cancels, leaving only the material density γ as a design variable.
The length of rod that is just on the verge of breaking under its own weight can now be found by letting
y = L (the highest stress occurs at the top), setting σ(L) = σf , and solving for L:
σf = γL ⇒ L =
In the case of steel, we ﬁnd the mass density ρ in Appendix A to be 7.85 × 103
1200 × 106
7.85 × 103(kg/m3) × 9.8(m/s2)
= 15.6 km
This would be a long rod indeed; the purpose of such a calculation is not so much to design superlong rods
as to provide a vivid way of comparing material.
1.2 Stiﬀness in Tension - Young’s Modulus
It is important to distinguish stiﬀness, which is a measure of the load needed to induce a given
deformation in the material, from the strength, which usually refers to the material’s resistance to
failure by fracture or excessive deformation. The stiﬀness is usually measured by applying relatively
small loads, well short of fracture, and measuring the resulting deformation. Since the deformations
in most materials are very small for these loading conditions, the experimental problem is largely
one of measuring small changes in length accurately.
Hooke3 made a number of such measurements on long wires under various loads, and observed
that to a good approximation the load P and its resulting deformation δ were related linearly as
long as the loads were suﬃciently small. This relation, generally known as Hooke’s Law, can be
written algebraically as
P = kδ (1.3)
where k is a constant of proportionality called the stiﬀness and having units of lb/in or N/m.
The stiﬀness as deﬁned by k is not a function of the material alone, but is also inﬂuenced by the
Robert Hooke (1635–1703) was a contemporary and rival of Isaac Newton. In the style of his time, Hooke
originally published his observation as a Latin anagram ceiiinossttuv from ut tensio, sic vis - As the extension, so the
1.2. STIFFNESS IN TENSION - YOUNG’S MODULUS 9
specimen shape. A wire gives much more deﬂection for a given load if coiled up like a watch spring,
A useful way to adjust the stiﬀness so as to be a purely materials property is to normalize the
load by the cross-sectional area; i.e. to use the tensile stress rather than the load. Further, the
deformation δ can be normalized by noting that an applied load stretches all parts of the wire
uniformly, so that a reasonable measure of “stretching” is the deformation per unit length:
Here L0 is the original length and is a dimensionless measure of stretching called the strain. Using
these more general measures of load per unit area and displacement per unit length4, Hooke’s Law
σ = E (1.6)
The constant of proportionality E, called Young’s modulus5 or the modulus of elasticity6, is one of
the most important mechanical descriptors of a material. It has the same units as stress, Pa or psi.
As shown in Fig. 1.5, Hooke’s law can refer to either of Eqns. 1.3 or 1.6.
Figure 1.5: Hooke’s law in terms of (a) load-displacement and (b) stress-strain.
The Hookean stiﬀness k is now recognizable as being related to the Young’s modulus E and the
specimen geometry as
It was apparently the Swiss mathematician Jakob Bernoulli (1655-1705) who ﬁrst realized the correctness of this
form, published in the ﬁnal paper of his life.
After the English physicist Thomas Young (1773–1829), who also made notable contributions to the understanding
of the interference of light as well as being a noted physician and Egyptologist.
Elasticity is a form of materials response that refers to immediate and time-independent deformation upon
loading, and complete and instant recovery of the original geometry upon removal of the load. A material is elastic
or it is not, one material cannot be “more elastic” than another, and a material can be elastic without obeying the
linear relation given by Hooke’s law.
10 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
where here the 0 subscript is dropped from the area A; it will be assumed from here on (unless
stated otherwise) that the change in area during loading can be neglected. Another useful relation
is obtained by solving Eqn. 1.5 for the deﬂection in terms of the applied load as
Note that the stress σ = P/A developed in a tensile specimen subjected to a ﬁxed load is in-
dependent of the material properties, while the deﬂection depends on the material property E.
Hence the stress σ in a tensile specimen at a given load is the same whether it’s made of steel or
polyethylene, but the strain would be diﬀerent: the polyethylene will exhibit much larger strain
and deformation, since its modulus is two orders of magnitude less than steel’s.
In Example 1.1, we found that a steel rod 0.38 in diameter would safely bear a load of 10,000 lb. Now let’s
assume we have been given a second design goal, namely that the geometry requires that we use a rod 15 ft
in length but that the loaded end cannot be allowed to deﬂect downward more than 0.3 when the load is
applied. Replacing A in Eqn. 1.8 by πd2
/4 and solving for d, the diameter for a given δ is
d = 2
From Appendix A, the modulus of carbon steel is 210 GPa; using this along with the given load, length, and
deﬂection, the required diameter is
d = 2
104(lb) × 15(ft) × 12(in/ft)
π × 0.3(in) × 210 × 109(N/m2) × 1.449 × 10−4 lb/in2
= 0.5 in
This diameter is larger than the 0.38 computed earlier; therefore a larger rod must be used if the
deﬂection as well as the strength goals are to be met. Clearly, using the larger rod makes the tensile stress
in the material less and thus lowers the likelihood of fracture. This is an example of a stiﬀness-critical
design, in which deﬂection rather than fracture is the governing constraint. As it happens, many structures
throughout the modern era have been designed for stiﬀness rather than strength, and thus wound up being
“overdesigned” with respect to fracture. This has undoubtedly lessened the incidence of fracture-related
catastrophes, which will be addressed in the chapters on fracture.
Figure 1.6: Deformation of a column under its own weight.
When very long columns are suspended from the top, as in a cable hanging down the hole of an oil well,
the deﬂection due to the weight of the material itself can be important. The solution for the total deﬂection
1.2. STIFFNESS IN TENSION - YOUNG’S MODULUS 11
is a minor extension of Eqn. 1.8, in that now we must consider the increasing weight borne by each cross
section as the distance from the bottom of the cable increases. As shown in Fig. 1.6, the total elongation of
a column of length L, cross-sectional area A, and weight density γ due to its own weight can be found by
considering the incremental deformation dδ of a slice dy a distance y from the bottom. The weight borne by
this slice is γAy, so
Note that δ is independent of the area A, so that ﬁnding a fatter cable won’t help to reduce the deformation;
the critical parameter is the speciﬁc modulus E/γ. Since the total weight is W = γAL, the result can also
The deformation is the same as in a bar being pulled with a tensile force equal to half its weight; this is just
the average force experienced by cross sections along the column.
In Example 2, we computed the length of a steel rod that would be just on the verge of breaking under
its own weight if suspended from its top; we obtained L = 15.6km. Were such a rod to be constructed, our
analysis predicts the deformation at the bottom would be
7.85 × 103
) × 9.8(m/s2
) × [15.6 × 103
2 × 210 × 109(N/m2)
= 44.6 m
However, this analysis assumes Hooke’s law holds over the entire range of stresses from zero to fracture. This
is not true for many materials, including carbon steel, and later chapters will address materials response at
A material that obeys Hooke’s Law (Eqn. 1.6) is called Hookean. Such a material is elastic
according to the description of elasticity given earlier (immediate response, full recovery), and it
is also linear in its relation between stress and strain (or equivalently, force and deformation).
Therefore a Hookean material is linear elastic, and materials engineers use these descriptors in-
terchangeably. It is important to keep in mind that not all elastic materials are linear (rubber is
elastic but nonlinear), and not all linear materials are elastic (viscoelastic materials can be linear
in the mathematical sense, but do not respond immediately and are thus not elastic).
The linear proportionality between stress and strain given by Hooke’s law is not nearly as general
as, say, Einstein’s general theory of relativity, or even Newton’s law of gravitation. It’s really just
an approximation that is observed to be reasonably valid for many materials as long the applied
stresses are not too large. As the stresses are increased, eventually more complicated material
response will be observed. Some of these eﬀects will be outlined in the later section on stress-strain
curves, which introduces the experimental measurement of the strain response of materials over a
range of stresses up to and including fracture.
If we were to push on the specimen rather than pulling on it, the loading would be described as
compressive rather than tensile. In the range of relatively low loads, Hooke’s law holds for this case
as well. By convention, compressive stresses and strains are negative, so the expression σ = E
holds for both tension and compression.
12 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
1.3 The Poisson Eﬀect
A positive (tensile) strain in one direction will also contribute a negative (compressive) strain in
the other direction, just as stretching a rubber band to make it longer in one direction makes it
thinner in the other directions (see Fig. 1.7). This lateral contraction accompanying a longitudinal
extension is called the Poisson eﬀect,7 and the Poisson’s ratio is a material property deﬁned as
where the minus sign accounts for the sign change between the lateral and longitudinal strains.
The stress-strain, or “constitutive,” law of the material must be extended to include these eﬀects,
since the strain in any given direction is inﬂuenced by not only the stress in that direction, but also
by the Poisson strains contributed by the stresses in the other two directions.
Figure 1.7: The Poisson eﬀect.
A material subjected only to a stress σx in the x direction will experience a strain in that
direction given by x = σx/E. A stress σy acting alone in the y direction will induce an x-direction
strain given from the deﬁnition of Poisson’s ratio of x = −ν y = −ν(σy/E). If the material is
subjected to both stresses σx and σy at once, the eﬀects can be superimposed (since the governing
equations are linear) to give:
(σx − νσy) (1.10)
Similarly for a strain in the y direction:
(σy − νσx) (1.11)
The material is in a state of plane stress if no stress components act in the third dimension (the
z direction, here). This occurs commonly in thin sheets loaded in their plane. The z components
of stress vanish at the surfaces because there are no forces acting externally in that direction to
balance them, and these components do not have suﬃcient specimen distance in the thin through-
thickness dimension to build up to appreciable levels. However, a state of plane stress is not a state
of plane strain. The sheet will experience a strain in the z direction equal to the Poisson strain
contributed by the x and y stresses:
z = −
(σx + σy) (1.12)
After the French mathematician Simeon Denis Poisson, (1781–1840).
1.4. SHEARING STRESSES AND STRAINS 13
The Poisson’s ratio is a dimensionless parameter that provides a good deal of insight into the
nature of the material. The major classes of engineered structural materials fall neatly into order
when ranked by Poisson’s ratio:
Class Ratio ν
(The values here are approximate.) It will be noted that the most brittle materials have the lowest
Poisson’s ratio, and that the materials appear to become generally more ﬂexible as the Poisson’s
ratio increases. The ability of a material to contract laterally as it is extended longitudinally is
related directly to its molecular mobility, with rubber being liquid-like and ceramics being very
The Poisson’s ratio is also related to the compressibility of the material. The bulk modulus K,
also called the modulus of compressibility, is the ratio of the hydrostatic pressure p needed for a
unit relative decrease in volume ∆V/V :
where the minus sign indicates that a compressive pressure (traditionally considered positive) pro-
duces a negative volume change. It can be shown that for isotropic materials the bulk modulus is
related to the elastic modulus and the Poisson’s ratio as
3(1 − 2ν)
This expression becomes unbounded as ν approaches 0.5, so that rubber is essentially incompress-
ible. Further, ν cannot be larger than 0.5, since that would mean volume would increase on the
application of positive pressure. A ceramic at the lower end of Poisson’s ratios, by contrast, is
so tightly bonded that it is unable to rearrange itself to “ﬁll the holes” that are created when a
specimen is pulled in tension; it has no choice but to suﬀer a volume increase. Paradoxically, the
tightly bonded ceramics have lower bulk moduli than the very mobile elastomers.
1.4 Shearing Stresses and Strains
Not all deformation is elongational or compressive, and we need to extend our concept of strain to
include “shearing,” or “distortional,” eﬀects. To illustrate the nature of shearing distortions, ﬁrst
consider a square grid inscribed on a tensile specimen as depicted in Fig. 1.8(a). Upon uniaxial
loading, the grid would be deformed so as to increase the length of the lines in the tensile loading
direction and contract the lines perpendicular to the loading direction. However, the lines remain
perpendicular to one another. These are termed normal strains, since planes normal to the loading
direction are moving apart.
Now consider the case illustrated in Fig. 1.8(b), in which the load P is applied transversely to
the specimen. Here the horizontal lines tend to slide relative to one another, with line lengths of the
originally square grid remaining unchanged. The vertical lines tilt to accommodate this motion, so
14 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
Figure 1.8: (a) Normal and (b) shearing deformations.
the originally right angles between the lines are distorted. Such a loading is termed direct shear.
Analogously to our deﬁnition of normal stress as force per unit area, or σ = P/A, we write the
shear stress τ as
This expression is identical to the expression for normal stress, but the diﬀerent symbol τ reminds
us that the loading is transverse rather than extensional.
Figure 1.9: Tongue-and-groove adhesive joint.
Two timbers, of cross-sectional dimension b × h, are to be glued together using a tongue-and-groove joint as
shown in Fig. 1.9, and we wish to estimate the depth d of the glue joint so as to make the joint approximately
as strong as the timber itself.
The axial load P on the timber acts to shear the glue joint, and the shear stress in the joint is just the
load divided by the total glue area:
If the bond fails when τ reaches a maximum value τf , the load at failure will be Pf = (2bd)τf . The load
needed to fracture the timber in tension is Pf = bhσf , where σf is the ultimate tensile strength of the timber.
Hence if the glue joint and the timber are to be equally strong we have
(2bd)τf = bhσf → d =
Normal stresses act to pull parallel planes within the material apart or push them closer together,
while shear stresses act to slide planes along one another. Normal stresses promote crack formation
and growth, while shear stresses underlie yield and plastic slip. The shear stress can be depicted
on the stress square as shown in Fig. 1.10(a); it is traditional to use a half-arrowhead to distinguish
1.4. SHEARING STRESSES AND STRAINS 15
Figure 1.10: Shear stress.
shear stress from normal stress. The yx subscript indicates the stress is on the y plane in the x
The τyx arrow on the +y plane must be accompanied by one in the opposite direction on the −y
plane, in order to maintain horizontal equilibrium. But these two arrows by themselves would tend
to cause a clockwise rotation, and to maintain moment equilibrium we must also add two vertical
arrows as shown in Fig. 1.10(b); these are labeled τxy, since they are on x planes in the y direction.
For rotational equilibrium, the magnitudes of the horizontal and vertical stresses must be equal:
τyx = τxy (1.15)
Hence any shearing that tends to cause tangential sliding of horizontal planes is accompanied by
an equal tendency to slide vertical planes as well. These stresses are positive by a sign convention
of + arrows on + faces being positive. A positive state of shear stress, then, has arrows meeting at
the upper right and lower left of the stress square. Conversely, arrows in a negative state of shear
meet at the lower right and upper left.
Figure 1.11: Shear strain.
The strain accompanying the shear stress τxy is a shear strain denoted γxy. This quantity is a
deformation per unit length just as was the normal strain , but now the displacement is transverse
to the length over which it is distributed (see Fig. 1.11). This is also the distortion or change in
the right angle:
= tan γ ≈ γ (1.16)
This angular distortion is found experimentally to be linearly proportional to the shear stress
at suﬃciently small loads, and the shearing counterpart of Hooke’s Law can be written as
τxy = Gγxy (1.17)
where G is a material property called the shear modulus. For isotropic materials (properties same
in all directions), there is no Poisson-type eﬀect to consider in shear, so that the shear strain
is not inﬂuenced by the presence of normal stresses. Similarly, application of a shearing stress
16 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
has no inﬂuence on the normal strains. For plane stress situations (no normal or shearing stress
components in the z direction), the constitutive equations as developed so far can be written:
x = 1
E (σx − νσy)
y = 1
E (σy − νσx)
γxy = 1
It will be shown later that for isotropic materials, only two of the material constants here are
independent, and that
2(1 + ν)
Hence if any two of the three properties E, G, or ν, are known, the other is determined.
1.5 Stress-Strain Curves
Stress-strain curves are an extremely important graphical measure of a material’s mechanical prop-
erties, and all students of Mechanics of Materials will encounter them often. However, they are
not without some subtlety, especially in the case of ductile materials that can undergo substantial
geometrical change during testing. This section will provide an introductory discussion of several
points needed to interpret these curves, and in doing so will also provide a preliminary overview
of several aspects of a material’s mechanical properties. However, this section will not attempt to
survey the broad range of stress-strain curves exhibited by modern engineering materials (the atlas
by Boyer cited in the References section can be consulted for this). Several of the topics mentioned
here — especially yield and fracture — will appear with more detail in later chapters.
1.5.1 “Engineering” Stress-Strain Curves
Perhaps the most important test of a material’s mechanical response is the tensile test8, in which one
end of a rod or wire specimen is clamped in a loading frame and the other subjected to a controlled
displacement δ (see Fig. 1.1). A transducer connected in series with the specimen provides an
electronic reading of the load P(δ) corresponding to the displacement. Alternatively, modern servo-
controlled testing machines permit using load rather than displacement as the controlled variable,
in which case the displacement δ(P) would be monitored as a function of load.
The engineering measures of stress and strain, denoted in this section as σe and e respectively,
are determined from the measured load and deﬂection using the original specimen cross-sectional
area A0 and length L0 as
, e =
When the stress σe is plotted against the strain e, an engineering stress-strain curve such as that
shown in Fig. 1.12 is obtained.
In the early (low strain) portion of the curve, many materials obey Hooke’s law to a reasonable
approximation, so that stress is proportional to strain with the constant of proportionality being
the modulus of elasticity or Young’s modulus E:
Stress-strain testing, as well as almost all experimental procedures in mechanics of materials, is detailed by
standards-setting organizations, notably the American Society for Testing and Materials (ASTM). Tensile testing of
metals is prescribed by ASTM Test E8, plastics by ASTM D638, and composite materials by ASTM D3039.
1.5. STRESS-STRAIN CURVES 17
Figure 1.12: Low-strain region of the engineering stress-strain curve for annealed polycrystaline
copper; this curve is typical of that of many ductile metals.
σe = E e (1.21)
As strain is increased, many materials eventually deviate from this linear proportionality, the
point of departure being termed the proportional limit. This nonlinearity is usually associated with
stress-induced “plastic” ﬂow in the specimen. Here the material is undergoing a rearrangement of
its internal molecular or microscopic structure, in which atoms are being moved to new equilibrium
positions. This plasticity requires a mechanism for molecular mobility, which in crystalline materials
can arise from dislocation motion (discussed further in a later chapter.) Materials lacking this
mobility, for instance by having internal microstructures that block dislocation motion, are usually
brittle rather than ductile. The stress-strain curve for brittle materials are typically linear over
their full range of strain, eventually terminating in fracture without appreciable plastic ﬂow.
Note in Fig. 1.12 that the stress needed to increase the strain beyond the proportional limit
in a ductile material continues to rise beyond the proportional limit; the material requires an
ever-increasing stress to continue straining, a mechanism termed strain hardening.
These microstructural rearrangements associated with plastic ﬂow are usually not reversed
when the load is removed, so the proportional limit is often the same as or at least close to the
material’s elastic limit. Elasticity is the property of complete and immediate recovery from an
imposed displacement on release of the load, and the elastic limit is the value of stress at which the
material experiences a permanent residual strain that is not lost on unloading. The residual strain
induced by a given stress can be determined by drawing an unloading line from the highest point
reached on the σ − curve at that stress back to the strain axis, drawn with a slope equal to that
of the initial elastic loading line. This is done because the material unloads elastically, there being
no force driving the molecular structure back to its original position.
A closely related term is the yield stress, denoted σY in this section; this is the stress needed to
induce plastic deformation in the specimen. Since it is often diﬃcult to pinpoint the exact stress at
which plastic deformation begins, the yield stress is often taken to be the stress needed to induce
a speciﬁed amount of permanent strain, typically 0.2%. The construction used to ﬁnd this “oﬀset
yield stress” is shown in Fig. 1.12, in which a line of slope E is drawn from the strain axis at
e = 0.2%; this is the unloading line that would result in the speciﬁed permanent strain. The stress
at the point of intersection with the σe − e curve is the oﬀset yield stress.
18 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
Figure 1.13 shows the engineering stress-strain curve for copper with an enlarged scale, now
showing strains from zero up to specimen fracture. Here it appears that the rate of strain hardening9
diminishes up to a point labeled UTS, for Ultimate Tensile Strength (denoted σf in this text).
Beyond that point, the material appears to strain soften, so that each increment of additional
strain requires a smaller stress.
Figure 1.13: Full engineering stress-strain curve for annealed polycrystalline copper.
The apparent change from strain hardening to strain softening is an artifact of the plotting
procedure, however, as is the maximum observed in the curve at the UTS. Beyond the yield point,
molecular ﬂow causes a substantial reduction in the specimen cross-sectional area A, so the true
stress σt = P/A actually borne by the material is larger than the engineering stress computed from
the original cross-sectional area (σe = P/A0). The load must equal the true stress times the actual
area (P = σtA), and as long as strain hardening can increase σt enough to compensate for the
reduced area A, the load and therefore the engineering stress will continue to rise as the strain
increases. Eventually, however, the decrease in area due to ﬂow becomes larger than the increase
in true stress due to strain hardening, and the load begins to fall. This is a geometrical eﬀect, and
if the true stress rather than the engineering stress were plotted no maximum would be observed
in the curve.
At the UTS the diﬀerential of the load P is zero, giving an analytical relation between the true
stress and the area at necking:
P = σtA → dP = 0 = σtdA + Adσt → −
The last expression states that the load and therefore the engineering stress will reach a maximum
as a function of strain when the fractional decrease in area becomes equal to the fractional increase
in true stress.
Even though the UTS is perhaps the materials property most commonly reported in tensile
tests, it is not a direct measure of the material due to the inﬂuence of geometry as discussed above,
and should be used with caution. The yield stress σY is usually preferred to the UTS in designing
with ductile metals, although the UTS is a valid design criterion for brittle materials that do not
exhibit these ﬂow-induced reductions in cross-sectional area.
The strain hardening rate is the slope of the stress-strain curve, also called the tangent modulus.
1.5. STRESS-STRAIN CURVES 19
The true stress is not quite uniform throughout the specimen, and there will always be some
location - perhaps a nick or some other defect at the surface - where the local stress is maximum.
Once the maximum in the engineering curve has been reached, the localized ﬂow at this site cannot
be compensated by further strain hardening, so the area there is reduced further. This increases
the local stress even more, which accelerates the ﬂow further. This localized and increasing ﬂow
soon leads to a “neck” in the gage length of the specimen such as that seen in Fig. 1.14.
Figure 1.14: Necking in a tensile specimen.
Until the neck forms, the deformation is essentially uniform throughout the specimen, but after
necking all subsequent deformation takes place in the neck. The neck becomes smaller and smaller,
local true stress increasing all the time, until the specimen fails. This will be the failure mode
for most ductile metals. As the neck shrinks, the nonuniform geometry there alters the uniaxial
stress state to a complex one involving shear components as well as normal stresses. The specimen
often fails ﬁnally with a “cup and cone” geometry as seen in Fig. 1.15, in which the outer regions
fail in shear and the interior in tension. When the specimen fractures, the engineering strain at
break — denoted f — will include the deformation in the necked region and the unnecked region
together. Since the true strain in the neck is larger than that in the unnecked material, the value of
f will depend on the fraction of the gage length that has necked. Therefore, f is a function of the
specimen geometry as well as the material, and thus is only a crude measure of material ductility.
Figure 1.15: Cup-and-cone fracture in a ductile metal.
Figure 1.16 shows the engineering stress-strain curve for a semicrystalline thermoplastic. The
response of this material is similar to that of copper seen in Fig. 1.13, in that it shows a proportional
limit followed by a maximum in the curve at which necking takes place. (It is common to term this
maximum as the yield stress in plastics, although plastic ﬂow has actually begun at earlier strains.)
The polymer, however, diﬀers dramatically from copper in that the neck does not continue
20 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
Figure 1.16: Stress-strain curve for polyamide (nylon) thermoplastic.
shrinking until the specimen fails. Rather, the material in the neck stretches only to a “natural
draw ratio” which is a function of temperature and specimen processing, beyond which the material
in the neck stops stretching and new material at the neck shoulders necks down. The neck then
propagates until it spans the full gage length of the specimen, a process called drawing. This
process can be observed without the need for a testing machine, by stretching a polyethylene
“six-pack holder,” as seen in Fig. 1.17.
Figure 1.17: Necking and drawing in a 6-pack holder.
Not all polymers are able to sustain this drawing process. As will be discussed in the next
section, it occurs when the necking process produces a strengthened microstructure whose breaking
load is greater than that needed to induce necking in the untransformed material just outside the
1.5.2 “True” Stress-Strain Curves
As discussed in the previous section, the engineering stress-strain curve must be interpreted with
caution beyond the elastic limit, since the specimen dimensions experience substantial change from
their original values. Using the true stress σt = P/A rather than the engineering stress σe = P/A0
can give a more direct measure of the material’s response in the plastic ﬂow range. A measure
of strain often used in conjunction with the true stress takes the increment of strain to be the
incremental increase in displacement dL divided by the current length L:
1.5. STRESS-STRAIN CURVES 21
d t =
→ t =
dL = ln
This is called the “true” or “logarithmic” strain.
During yield and the plastic-ﬂow regime following yield, the material ﬂows with negligible change
in volume; increases in length are oﬀset by decreases in cross-sectional area. Prior to necking, when
the strain is still uniform along the specimen length, this volume constraint can be written:
dV = 0 → AL = A0L0 →
The ratio L/L0 is the extension ratio, denoted as λ. Using these relations, it is easy to develop
relations between true and engineering measures of tensile stress and strain:
σt = σe (1 + e) = σeλ, t = ln (1 + e) = ln λ (1.25)
These equations can be used to derive the true stress-strain curve from the engineering curve, up to
the strain at which necking begins. Figure 1.18 is a replot of Fig. 1.13, with the true stress-strain
curve computed by this procedure added for comparison.
Figure 1.18: Comparison of engineering and true stress-strain curves for copper. An arrow indicates
the position on the “true” curve of the UTS on the engineering curve.
Beyond necking, the strain is nonuniform in the gage length and to compute the true stress-
strain curve for greater engineering strains would not be meaningful. However, a complete true
stress-strain curve could be drawn if the neck area were monitored throughout the tensile test, since
for logarithmic strain we have
→ t = ln
Ductile metals often have true stress-strain relations that can be described by a simple power-law
relation of the form:
σt = A n
t → log σt = log A + n log t (1.27)
22 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
Figure 1.19 is a log-log plot of the true stress-strain data10 for copper from Fig. 1.18 that demon-
strates this relation. Here the parameter n = 0.474 is called the strain hardening parameter, useful
as a measure of the resistance to necking. Ductile metals at room temperature usually exhibit
values of n from 0.02 to 0.5.
Figure 1.19: Power-law representation of the plastic stress-strain relation for copper.
The increase in strain hardening rate needed to sustain the drawing process in semicrystalline
polymers arises from a dramatic transformation in the material’s microstructure. These materials
are initially “spherulitic,” containing ﬂat lamellar crystalline plates, perhaps 10 nm thick, arranged
radially outward in a spherical domain. As the induced strain increases, these spherulites are ﬁrst
deformed in the straining direction. As the strain increases further, the spherulites are broken apart
and the lamellar fragments rearranged with a dominantly axial molecular orientation to become
what is known as the ﬁbrillar microstructure. With the strong covalent bonds now dominantly lined
up in the load-bearing direction, the material exhibits markedly greater strengths and stiﬀnesses
— by perhaps an order of magnitude — than in the original material. This structure requires a
much higher strain hardening rate for increased strain, causing an upturn in the true stress-strain
The above discussion is concerned primarily with simple tension, i.e. uniaxial loading that increases
the interatomic spacing. However, as long as the loads are suﬃciently small (stresses less than the
proportional limit), in many materials the relations outlined above apply equally well if loads
are placed so as to put the specimen in compression rather than tension. The expression for
deformation and a given load δ = PL/AE applies just as in tension, with negative values for δ
and P indicating compression. Further, the modulus E is the same in tension and compression to
a good approximation, and the stress-strain curve simply extends as a straight line into the third
quadrant as shown in Fig. 1.20.
There are some practical diﬃculties in performing stress-strain tests in compression. If exces-
sively large loads are mistakenly applied in a tensile test, perhaps by wrong settings on the testing
machine, the specimen simply breaks and the test must be repeated with a new specimen. But in
Here percent strain was used for t; this produces the same value for n but a diﬀerent A than if full rather than
percentage values were used.
1.6. PROBLEMS 23
Figure 1.20: Stress-strain curve in tension and compression.
compression, a mistake can easily damage the load cell or other sensitive components, since even
after specimen failure the loads are not necessarily relieved.
Specimen failure by cracking is inhibited in compression, since cracks will be closed up rather
than opened by the stress state. A number of important materials are much stronger in compression
than in tension for this reason. Concrete, for example, has good compressive strength and so ﬁnds
extensive use in construction in which the dominant stresses are compressive. But it has essentially
no strength in tension, as cracks in sidewalks and building foundations attest: tensile stresses appear
as these structures settle, and cracks begin at very low tensile strain in unreinforced concrete.
1. Determine the stress and total deformation of an aluminum wire, 30 m long and 5 mm in diameter,
subjected to an axial load of 250 N.
2. A tapered column of modulus E and mass density ρ varies linearly from a radius of r1 to r2 in a length
L, and is hanging from its broad end. Find the total deformation due to the weight of the bar.
3. The ﬁgure below shows the engineering stress-strain curve for pure polycrystalline aluminum; the
numerical data for this ﬁgure are in the ﬁle http://web.mit.edu/course/3/3.225/alum.txt, which
can be imported into a spreadsheet or other analysis software. For this material, determine (a) Young’s
modulus, (b) the 0.2% oﬀset yield strength, (c) the Ultimate Tensile Strength (UTS), (d) the modulus
of resilience, and (e) the modulus of toughness.
24 CHAPTER 1. UNIAXIAL MECHANICAL RESPONSE
1. Ashby, M., et al., Materials: Engineering, Science, Processing and Design, Elsevier, Amsterdam. 2007.
2. Boyer, H.F., Atlas of Stress-Strain Curves, ASM International, Metals Park, Ohio, 1987.
3. Courtney, T.H., Mechanical Behavior of Materials, McGraw-Hill, New York, 1990.
4. Hayden, H.W., W.G. Moﬀatt and J. Wulﬀ, The Structure and Properties of Materials: Vol. III
Mechanical Behavior, Wiley, New York, 1965.
5. Jenkins, C. and S. Khanna, Mechanics of Materials, Elsevier, Amsterdam, 2005.
Thermodynamics of Mechanical
The ﬁrst law of thermodynamics states that an input of heat dQ or mechanical work dW to a system leads
to a change in internal energy dU according to dU = dW + dQ. For a reversible process the second law
gives dQ = T dS, and we will be concerned with increments of mechanical work in the form dW = f dx.
Combining these relations gives
f dx = dU − T dS (2.1)
Hence an increment of mechanical work f dx done on the system can produce an increase in the internal
energy dU or a decrease in the entropy dS. We will be concerned in this chapter ﬁrst with materials of limited
mobility that are unable to exhibit entropic conﬁgurational changes, so the response is solely enthalpic. We
will then treat materials that are so mobile we can neglect the enthalpic component in comparison with the
entropy change. Finally we will consider viscoelastic materials that exhibit appreciable amounts of both
enthalpic and entropic eﬀects in their response.
2.1 Enthalpic Response
For most materials, the amount of stretching experienced by a tensile specimen under a small ﬁxed load
is controlled in a relatively simple way by the tightness of the chemical bonds at the atomic level, and
this makes it possible to relate stiﬀness to the chemical architecture of the material. This is in contrast to
more complicated mechanical properties such as fracture, which are controlled by a diverse combination of
microscopic as well as molecular aspects of the material’s internal structure and surface. Further, the stiﬀness
of some materials — notably rubber — arises not from bond stiﬀness but from disordering or entropic factors.
2.1.1 The Bond Energy Function
Chemical bonding between atoms can be viewed as arising from the electrostatic attraction between regions of
positive and negative electronic charge. Materials can be classiﬁed based on the nature of these electrostatic
forces, the three principal classes being
1. Ionic materials, such as NaCl, in which an electron is transferred from the less electronegative element
(Na) to the more electronegative (Cl). The ions therefore diﬀer by one electronic charge and are thus
attracted to one another. Further, the two ions feel an attraction not only to each other but also to
other oppositely charged ions in their vicinity; they also feel a repulsion from nearby ions of the same
charge. Some ions may gain or lose more than one electron.
2. Metallic materials, such as iron and copper, in which one or more loosely bound outer electrons are
released into a common pool which then acts to bind the positively charged atomic cores.
26 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
3. Covalent materials, such as diamond and polyethylene, in which atomic orbitals overlap to form a
region of increased electronic charge to which both nuclei are attracted. This bond is directional, with
each of the nuclear partners in the bond feeling an attraction to the negative region between them but
not to any of the other atoms nearby.
In the case of ionic bonding, Coulomb’s law of electrostatic attraction can be used to develop simple but
eﬀective relations for the bond stiﬀness. For ions of equal charge e the attractive force fattr can be written:
Here C is a conversion factor; For e in Coulombs, C = 8.988 × 109
. For singly ionized atoms,
e = 1.602 × 10−19
Coul is the charge on an electron. The energy associated with the Coulombic attraction
is obtained by integrating the force, which shows that the bond energy varies inversely with the separation
Uattr = fattr dr =
where the energy of atoms at inﬁnite separation is taken as zero.
Figure 2.1: The interpenetrating cubic NaCl lattice.
If the material’s atoms are arranged as a perfect crystal, it is possible to compute the electrostatic
binding energy ﬁeld in considerable detail. In the interpenetrating cubic lattice of the ionic NaCl structure
shown in Fig. 2.1, for instance, each ion feels attraction to oppositely charged neighbors and repulsion from
equally charged ones. A particular sodium atom is surrounded by 6 Cl−
ions at a distance r, 12 Na+
at a distance r
2, 8 Cl−
ions at a distance r
3, etc. The total electronic ﬁeld sensed by the ﬁrst sodium
ion is then:
Uattr = −
− · · · (2.4)
where A = 1.747558 · · · is the result of the previous series, called the Madelung constant1
. Note that it is
not suﬃcient to consider only nearest-neighbor attractions in computing the bonding energy; in fact the
second term in the series is larger in magnitude than the ﬁrst. The speciﬁc value for the Madelung constant
is determined by the crystal structure, being 1.763 for CsCl and 1.638 for cubic ZnS.
C. Kittel, Introduction to Solid State Physics, John Wiley & Sons, New York, 1966. The Madelung series does
not converge smoothly, and this text includes some approaches to computing the sum.
2.1. ENTHALPIC RESPONSE 27
At close separation distances, the attractive electrostatic force is balanced by mutual repulsion forces
that arise from interactions between overlapping electron shells of neighboring ions; this force varies much
more strongly with the distance, and can be written:
Compressibility experiments have determined the exponent n to be 7.8 for the NaCl lattice, so this is a much
steeper function than Uattr.
Figure 2.2: The bond energy function.
As shown in Fig. 2.2, the total binding energy of one ion due to the presence of all others is then the
sum of the attractive and repulsive components:
U = −
Note that the curve is anharmonic (not shaped like a sine curve), being more ﬂattened out at larger separation
distances. The system will adopt a conﬁguration near the position of lowest energy, computed by locating
the position of zero slope in the energy function:
The range for n is generally 5–12, increasing as the number of outer-shell electrons that cause the repulsive
In practice the n and B parameters in Eqn. 2.6 are determined from experimental measurements, for
instance by using a combination of X-ray diﬀraction to measure r0 and elastic modulus to infer the slope of
the U(r) curve. As an illustration of this process, picture a tensile stress σ applied to a unit area of crystal
(A = 1) as shown in Fig. 2.3, in a direction perpendicular to the crystal cell face. The total force on this
unit area is numerically equal to the stress: F = σA = σ.
If the interionic separation is r0, there will be 1/r2
0 ions on the unit area, each being pulled by a force f.
Since the total force F is just f times the number of ions, the stress can then be written
28 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
Figure 2.3: Simple tension applied to crystal face.
σ = F = f
When the separation between two adjacent ions is increased by an amount δ, the strain is = δ/r0. The
diﬀerential strain corresponding to a diﬀerential displacement is then
The elastic modulus E is now the ratio of stress to strain, in the limit as the strain approaches zero:
Using B = ACe2
0 /n from Eqn. 2.7 and simplifying,
(n − 1)ACe2
Note the very strong dependence of E on r0, which in turn reﬂects the tightness of the bond. If E and r0
are known experimentally, n can be determined. For NaCl, E = 3 × 1010
; using this along with the
X-ray diﬀraction value of r0 = 2.82 × 10−10
m, we ﬁnd n = 1.47.
Using simple tension in this calculation is not really appropriate, because when a material is stretched
in one direction, it will contract in the transverse directions. This is the Poisson eﬀect, discussed in the
previous chapter. Our tension-only example does not consider the transverse contraction, and the resulting
value of n is too low. A better but slightly more complicated approach is to use hydrostatic compression,
which moves all the ions closer to one another.
The stiﬀnesses of metallic and covalent systems will be calculated diﬀerently than the method
used above for ionic crystals, but the concept of electrostatic attraction applies to these non-ionic
systems as well. As a result, bond energy functions of a qualitatively similar nature result from all
these materials. In general, the “tightness” of the bond, and hence the elastic modulus E, is related
to the curvature of the bond energy function. Steeper bond functions will also be deeper as a rule,
so that within similar classes of materials the modulus tends to correlate with the energy needed to
rupture the bonds, for instance by melting. Materials such as tungsten that ﬁll many bonding and
few antibonding orbitals have very deep bonding functions2, with correspondingly high stiﬀnesses
The cohesive energy of materials is an important topic in solid state physics; see for example J. Livingston,
Electronic Properties of Engineering Materials, Wiley, 1999.
2.1. ENTHALPIC RESPONSE 29
Figure 2.4: Bond energy functions for aluminum and tungsten.
and melting temperatures, as illustrated in Fig. 2.4. This correlation is obvious in Table 2.1, which
lists the values of modulus for a number of metals, along with the values of melting temperature
Tm and melting energy ∆H.
Table 2.1: Modulus and bond strengths for transition metals.
Material E Tm ∆H αL
GPa (Mpsi) ◦C kJ/mol ×10−6,◦ C−1
Pb 14 (2) 327 5.4 29
Al 69 (10) 660 10.5 22
Cu 117 (17) 1084 13.5 17
Fe 207 (30) 1538 15.3 12
W 407 (59) 3410 32 4.2
2.1.2 Thermal Expansion
The system will generally have suﬃcient thermal energy to reside at a level somewhat above the
minimum in the bond energy function, and will oscillate between the two positions labeled A and
B in Fig. 2.5, with an average position near r0. This simple idealization provides a rationale for
why materials expand when the temperature is raised. As the internal energy is increased by the
addition of heat, the system oscillates between the positions labeled A and B with an average
separation distance r0. Since the curve is anharmonic, the average separation distance is now
greater than before, so the material has expanded or stretched. To a reasonable approximation,
the relative thermal expansion ∆L/L is often related linearly to the temperature rise ∆T, and we
= T = αL ∆T (2.8)
where T is a thermal strain and the constant of proportionality αL is the coeﬃcient of linear
thermal expansion. The expansion coeﬃcient αL will tend to correlate with the depth of the energy
curve, as is seen in Table 2.1.
30 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
Figure 2.5: Anharmonicity of the bond energy function.
A steel bar of length L and cross-sectional area A is ﬁtted snugly between rigid supports as shown in
Fig. 2.6. We wish to ﬁnd the compressive stress in the bar when the temperature is raised by an amount
Figure 2.6: Bar between rigid supports.
If the bar were free to expand, it would increase in length by an amount given by Eqn. 2.8. Clearly,
the rigid supports have to push on the bar – i.e. put in into compression – to suppress this expansion. The
magnitude of this thermally induced compressive stress could be found by imagining the material free to
expand, then solving σ = E T for the stress needed to “push the material back” to its unstrained state.
Equivalently, we could simply set the sum of a thermally induced strain and a mechanical strain σ to zero:
= σ + T =
+ αL∆T = 0
σ = −αLE∆T
The minus sign in this result reminds us that a negative (compressive) stress is induced by a positive
temperature change (temperature rises.)
A glass container of stiﬀness E and thermal expansion coeﬃcient αL is removed from a hot oven and plunged
suddenly into cold water. We know from experience that this “thermal shock” could fracture the glass, and
we’d like to see what materials parameters control this phenomenon. The analysis is very similar to that of
the previous example.
In the time period just after the cold-water immersion, before signiﬁcant heat transfer by conduction
can take place, the outer surfaces of the glass will be at the temperature of the cold water while the interior
2.1. ENTHALPIC RESPONSE 31
is still at the temperature of the oven. The outer surfaces will try to contract, but are kept from doing so
by the still-hot interior; this causes a tensile stress to develop on the surface. As before, the stress can be
found by setting the total strain to zero:
= σ + T =
+ αL∆T = 0
σ = −αLE∆T
Here the temperature change ∆T is negative if the glass is going from hot to cold, so the stress is positive
(tensile). If the glass is not to fracture by thermal shock, this stress must be less than the ultimate tensile
strength σf ; hence the maximum allowable temperature diﬀerence is
To maximize the resistance to thermal shock, the glass should have as low a value of αLE as possible.
“Pyrex” glass was developed speciﬁcally for improved thermal shock resistance by using boron rather than
soda and lime as process modiﬁers; this yields a much reduced value of αL.
Material properties for a number of important structural materials are listed in the Module on
Material Properties. When the column holding Young’s Modulus is plotted against the column
containing the Thermal Expansion Coeﬃcients (using log-log coordinates), the graph shown in
Fig. 2.7 is obtained. Here we see again the general inverse relationship between stiﬀness and
thermal expansion, and the distinctive nature of polymers is apparent as well.
Figure 2.7: Correlation of stiﬀness and thermal expansion for materials of various types.
Not all types of materials can be described by these simple bond-energy concepts: intramolecular
polymer covalent bonds have energies entirely comparable with ionic or metallic bonds, but most
common polymers have substantially lower moduli than most metals or ceramics. This is due to the
intermolecular bonding in polymers being due to secondary bonds which are much weaker than the
strong intramolecular covalent bonds. Polymers can also have substantial entropic contributions to
their stiﬀness, as will be described below, and these eﬀects do not necessarily correlate with bond
32 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
2.2 Entropic Response
The internal energy as given by the function U(r) is suﬃcient to determine the atomic positions in
many engineering materials; the material “wants” to minimize its internal energy, and it does this
by optimizing the balance of attractive and repulsive electrostatic bonding forces. But when the
absolute temperature is greater than approximately two-thirds of the melting temperature, there
can be suﬃcient molecular mobility that entropic or disordering eﬀects must be considered as well.
This is often the case for polymers even at room temperature, due to their weak intermolecular
When the temperature is high enough, polymer molecules can be viewed as an interpenetrating
mass of (extremely long) wriggling worms, constantly changing their positions by rotation about
carbon-carbon single bonds. This wriggling does not require straining the bond lengths or angles,
and large changes in position are possible with no change in internal bonding energy.
Figure 2.8: Conformational change in polymers.
The shape, or “conformation” of a polymer molecule can range from a fully extended chain to
a randomly coiled sphere (see Fig. 2.8). Statistically, the coiled shape is much more likely than
the extended one, simply because there are so many ways the chain can be coiled and only one
way it can be fully extended. In thermodynamic terms, the entropy of the coiled conformation
is very high (many possible “microstates”), and the entropy of the extended conformation is very
low (only one possible microstate). If the chain is extended and then released, there will be more
wriggling motions tending to the most probable state than to even more highly stretched states; the
material would therefore shrink back to its unstretched and highest-entropy state. Equivalently, a
person holding the material in the stretched state would feel a tensile force as the material tries
to unstretch and is prevented from doing so. These eﬀects are due to entropic factors, and not
internal bond energy.
It is possible for materials to exhibit both internal energy and entropic elasticity. Energy eﬀects
dominate in most materials, but rubber is much more dependent on entropic eﬀects. An ideal
rubber is one in which the response is completely entropic, with the internal energy changes being
When we stretch a rubber band, the molecules in its interior become extended because they
are crosslinked by chemical or physical junctions as shown in Fig. 2.9. Without these links, the
molecules could simply slide past one another with little or no uncoiling. “Silly Putty ” is an
example of uncrosslinked polymer, and its lack of junction connections cause it to be a viscous ﬂuid
rather than a useful elastomer that can bear sustained loads without continuing ﬂow. The crosslinks
provide a means by which one molecule can pull on another, and thus establish load transfer within
the materials. They also have the eﬀect of limiting how far the rubber can be stretched before
breaking, since the extent of the entropic uncoiling is limited by how far the material can extend
before pulling up tight against the network of junction points. We will see below that the stiﬀness
of a rubber can be controlled directly by adjusting the crosslink density, and this is an example of
2.2. ENTROPIC RESPONSE 33
process-structure-property control in materials.
Figure 2.9: Stretching of crosslinked or entangled polymers.
As the temperature is raised, the Brownian-type wriggling of the polymer is intensiﬁed, so that
the material seeks more vigorously to assume its random high-entropy state. This means that
the force needed to hold a rubber band at ﬁxed elongation increases with increasing temperature.
Similarly, if the band is stretched by hanging a ﬁxed weight on it, the band will shrink as the
temperature is raised. In some thermodynamic formalisms it is convenient to model this behavior
by letting the coeﬃcient of thermal expansion be a variable parameter, with the ability to become
negative for suﬃciently large tensile strains. This is a little tricky, however; for instance, the
stretched rubber band will contract only along its long axis when the temperature is raised, and
will become thicker in the transverse directions. The coeﬃcient of thermal expansion would have
to be made not only stretch-dependent but also dependent on direction (“anisotropic”).
It is worthwhile to study the response of rubbery materials in some depth, partly because this
provides a broader view of the elasticity of materials. But this isn’t a purely academic goal. Rubbery
materials are being used in increasingly demanding mechanical applications (in addition to tires,
which is a very demanding application itself). Elastomeric bearings, vibration-control supports, and
biomedical prostheses are but a few examples. We will outline what is known as the “kinetic theory
of rubber elasticity,” which treats the entropic eﬀect using concepts of statistical thermodynamics.
This theory stands as one of the very most successful atomistic theories of mechanical response. It
leads to a result of satisfying accuracy without the need for adjustable parameters or other fudge
From Eqn. 2.1 we have
For an ideal rubber, the enthalpy change dU is negligible, so the force is related directly to the
temperature and the change in entropy dS accompanying the extension dx.
To determine the force-deformation relationship, we obviously need to consider how S changes
with deformation. We begin by writing an expression for the conformation, or shape, of the segment
of polymer molecule between junction points as a statistical probability distribution. Here the
length of the segment is the important molecular parameter, not the length of the entire molecule.
In the simple form of this theory, which turns out to work quite well, each covalently bonded
segment is idealized as a freely-jointed sequence of n rigid links each having length a.
A reasonable model for the end-to-end distance of a randomly wriggling segment is that of a
34 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
Figure 2.10: Random-walk model of polymer conformation
“random walk” Gaussian distribution treated in elementary statistics. One end of the chain is
visualized at the origin of an xyz coordinate system as shown in Fig. 2.10, and each successive link
in the chain is attached with a random orientation relative to the previous link. (An elaboration
of the theory would constrain the orientation so as to maintain the 109◦ covalent bonding angle.)
The probability Ω1(r) that the other end of the chain is at a position r = x2 + y2 + z2 1/2
shown to be
The parameter β is a scale factor related to the number of units n in the polymer segment and the
bond length a; speciﬁcally it turns out that β = 3/2n/a. This is the “bell-shaped curve” well
known to seasoned test-takers. The most probable end-to-end distance is seen to be zero, which is
expected because the chain will end up a given distance to the left (or up, or back) of the origin
exactly as often as it ends up the same distance to the right.
When the molecule is now stretched or otherwise deformed, the relative positions of the two
ends are changed. Deformation in elastomers is usually described in terms of extension ratios, which
are the ratios of stretched to original dimensions, L/L0. Stretches in the x, y, and z directions are
denoted by λx, λy, and λz respectively, The deformation is assumed to be aﬃne, i.e. the end-to-end
distances of each molecular segment increase by these same ratios. Hence if we continue to view
one end of the chain at the origin the other end will have moved to x2 = λxx, y2 = λyy, z2 = λzz.
The conﬁgurational probability of a segment being found in this stretched state is then
The relative change in probabilities between the perturbed and unperturbed states can now be
x − 1 x2
y − 1 y2
z − 1 z2
Several strategems have been used in the literature to simplify this expression. One simple approach
is to let the initial position of the segment end x, y, z be such that x2 = y2 = z2 = r2
0/3, where r2
the initial mean square end-to-end distance of the segment. (This is not zero, since when squares
are taken the negative values no longer cancel the positive ones.) It can also be shown that the
0 is related to the number of bonds n in the segment and the bond length a by r2
0 = na2.
Making these substitutions and simplifying, we have
x + λ2
y + λ2
z − 3 (2.10)
2.2. ENTROPIC RESPONSE 35
As is taught in subjects in statistical thermodynamics, changes in conﬁgurational probability are
related to corresponding changes in thermodynamic entropy by the “Boltzman relation” as
∆S = k ln
where k = 1.38 × 10−23 J/K is Boltzman’s constant. Substituting Eqn. 2.10 in this relation:
∆S = −
x + λ2
y + λ2
z − 3
This is the entropy change for one segment. If there are N chain segments per unit volume, the
total entropy change per unit volume ∆SV is just N times this quantity:
∆SV = −
x + λ2
y + λ2
z − 3 (2.11)
The associated work (per unit volume) required to change the entropy by this amount is
∆WV = −T∆SV = +
x + λ2
y + λ2
z − 3 (2.12)
The quantity ∆WV is therefore the strain energy per unit volume contained in an ideal rubber
stretched by λx, λy, λz.
To illustrate the use of Eqn. 2.12 for a simple but useful case, consider a rubber band, initially
of length L0 which is stretched to a new length L. Hence λ = λx = L/L0. To a very good
approximation, rubbery materials maintain a constant volume during deformation, and this lets us
compute the transverse contractions λy and λz which accompany the stretch λx. An expression
for the change ∆V in a cubical volume of initial dimensions a0, b0, c0 which is stretched to new
dimensions a, b, c is
∆V = abc − a0b0c0 = (a0λx)(b0λy)(c0λz) − a0b0c0 = a0b0c0(λxλyλz − 1)
Setting this to zero gives
λxλyλz = 1 (2.13)
Hence the contractions in the y and z directions are
y = λ2
Using this in Eqn. 2.12, the force F needed to induce the deformation can be found by diﬀerentiating
the total strain energy according to Eqn. 2.9:
d(V ∆WV )
Here A0 = V/L0 is the original area. Dividing by A0 to obtain the engineering stress:
σ = NkT λ −
36 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
Clearly, the parameter NkT is related to the stiﬀness of the rubber, as it gives the stress σ needed
to induce a given extension λ. It can be shown that the initial modulus — the slope of the stress-
strain curve at the origin — is controlled by the temperature and the crosslink density according
to E = 3NkT.
Crosslinking in rubber is usually done in the “vulcanizing” process invented by Charles Goodyear
in 1839. In this process sulfur abstracts reactive hydrogens adjacent to the double bonds in the
rubber molecule, and forms permanent bridges between adjacent molecules. When crosslinking is
done by using approximately 5% sulfur, a conventional rubber is obtained. When the sulfur is
increased to ≈ 30–50%, a hard and brittle material named ebonite (or simply “hard rubber”) is
The volume density of chain segments N is also the density of junction points. This quantity is
related to the specimen density ρ and the molecular weight between crosslinks Mc as Mc = ρNA/N,
where N is the number of crosslinks per unit volume and NA = 6.023×1023 is Avogadro’s Number.
When N is expressed in terms of moles per unit volume, we have simply Mc = ρ/N and the quantity
NkT in Eqn. 2.14 is replaced by NRT, where R = kNA = 8.314 J/mol-◦K is the Gas Constant.
The Young’s modulus of a rubber is measured at E = 3.5 MPa for a temperature of T = 300 ◦
K. The molar
crosslink density is then
3.5 × 106
3 × 8.314 N·m
mol·K × 300 K
= 468 mol/m3
The molecular weight per segment is
= 2350 gm/mol
Note that the stress-strain response for rubber elasticity is nonlinear, and that the stiﬀness as
given by the stress needed to produce a given deformation is predicted to increase with increasing
temperature. This is in accord with the concept of more vigorous wriggling with a statistical bias
toward the more disordered state. The rubber elasticity equation works well at lower extensions,
but tends to deviate from experimental values at high extensions where the segment conﬁgurations
Deviations from Eqn. 2.14 can also occur due to crystallization at high elongations. (Rubbers
are normally noncrystalline, and in fact polymers such as polyethylene that crystallize readily are
not elastomeric due to the rigidity imparted by the crystallites.) However, the decreased entropy
that accompanies stretching in rubber increases the crystalline melting temperature according to
the well-known thermodynamic relation
where ∆U and ∆S are the change in internal energy and entropy on crystallization. The quantity
∆S is reduced if stretching has already lowered the entropy, so the crystallization temperature rises.
If it rises above room temperature, the rubber develops crystallites that stiﬀen it considerably and
cause further deviation from the rubber elasticity equation. (Since the crystallization is exothermic,
the material will also increase in temperature; this can often be sensed by stretching a rubber band
and then touching it to the lips.) Strain-induced crystallization also helps inhibit crack growth, and
the excellent abrasion resistance of natural rubber is related to the ease with which it crystallizes
2.3. VISCOELASTICITY 37
As mentioned at the outset of this chapter, some materials exhibit a combination of enthalpic and
entropic mechanical response. “Viscoelastic” polymers are an example, in which an immediate and
recoverable response due to bond distortion can take place, but also accompanied by an entropic
response due to conformational change.
While not all polymers are viscoelastic to any important practical extent, and even fewer are
linearly viscoelastic3, the linear theory provides a usable engineering approximation for many ap-
plications in polymer and composites engineering. Even in instances requiring more elaborate
treatments, the linear viscoelastic theory is a useful starting point.
2.3.1 Rate of Conformational Change
When subjected to an applied stress, polymers may deform by either or both of two fundamentally
diﬀerent atomistic mechanisms. The lengths and angles of the chemical bonds connecting the atoms
may distort, moving the atoms to new positions of greater internal energy. This is a small motion
and occurs very quickly, requiring only ≈ 10−12 seconds.
If the polymer has suﬃcient molecular mobility, larger-scale rearrangements of the atoms may
also be possible. For instance, the relatively facile rotation around backbone carbon-carbon single
bonds can produce large changes in the conformation of the molecule. Depending on the mobility,
a polymer molecule can extend itself in the direction of the applied stress, which decreases its
conformational entropy (the molecule is less “disordered”). Elastomers — rubber — respond almost
wholly by this entropic mechanism, with little distortion of their covalent bonds or change in their
In contrast to the instantaneous nature of the energetically controlled elasticity, the conforma-
tional or entropic changes are processes whose rates are sensitive to the local molecular mobility.
This mobility is inﬂuenced by a variety of physical and chemical factors, such as molecular archi-
tecture, temperature, or the presence of absorbed ﬂuids which may swell the polymer. Often, a
simple mental picture of “free volume” — roughly, the space available for molecular segments to
act cooperatively so as to carry out the motion or reaction in question — is useful in intuiting these
These rates of conformational change can often be described with reasonable accuracy by
Arrhenius-type expressions of the form
rate ∝ exp
where E† is an apparent activation energy of the process and R = 8.314J/mol − ◦K is the Gas
Constant. At temperatures much above the “glass transition temperature,” labeled Tg in Fig. 2.11,
the rates are so fast as to be essentially instantaneous, and the polymer acts in a rubbery manner in
which it exhibits large, instantaneous, and fully reversible strains in response to an applied stress.
Conversely, at temperatures much less than Tg, the rates are so slow as to be negligible. Here
the chain uncoiling process is essentially “frozen out,” so the polymer is able to respond only by
bond stretching. It now responds in a “glassy” manner, responding instantaneously and reversibly
but being incapable of being strained beyond a few percent before fracturing in a brittle manner.
In the range near Tg, the material is midway between the glassy and rubbery regimes. Its re-
sponse is a combination of viscous ﬂuidity and elastic solidity, and this region is termed “leathery,”
For an overview of nonlinear viscoelastic theory, see for instance W.N. Findley et al., Creep and Relaxation of
Nonlinear Viscoelastic Materials, Dover Publications, New York, 1989.
38 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
Figure 2.11: Temperature dependence of rate.
or, more technically, “viscoelastic”. The value of Tg is an important descriptor of polymer ther-
momechanical response, and is a fundamental measure of the material’s propensity for mobility.
Factors that enhance mobility, such as absorbed diluents, expansive stress states, and lack of bulky
molecular groups, all tend to produce lower values of Tg. The transparent polyvinyl butyral ﬁlm
used in automobile windshield laminates is an example of a material that is used in the viscoelastic
regime, as viscoelastic response can be a source of substantial energy dissipation during impact.
At temperatures well below Tg, when entropic motions are frozen and only elastic bond de-
formations are possible, polymers exhibit a relatively high modulus, called the “glassy modulus”
Eg, which is on the order of 3 GPa (400 kpsi). As the temperature is increased through Tg, the
stiﬀness drops dramatically, by perhaps two orders of magnitude, to a value called the “rubbery
modulus” Er. In elastomers that have been permanently crosslinked by sulphur vulcanization or
other means, the value of Er is determined primarily by the crosslink density; the kinetic theory of
rubber elasticity described in the previous section gave this value as Er = 3NRT.
If the material is not crosslinked, the stiﬀness exhibits a short plateau due to the ability of
molecular entanglements to act as network junctions; at still higher temperatures the entanglements
slip and the material becomes a viscous liquid. Neither the glassy nor the rubbery modulus depends
strongly on time, but in the vicinity of the transition near Tg time eﬀects can be very important.
Clearly, a plot of modulus versus temperature, such as is shown in Fig. 2.12, is a vital tool in
polymer materials science and engineering. It provides a map of a vital engineering property, and
is also a ﬁngerprint of the molecular motions available to the material.
2.3.2 Creep Compliance
In the viscoelastic range where the entropic conﬁgurational change is neither so slow as to be
negligible or so rapid as to be essentially immediate, the material exhibits a “delayed” mechanical
response; this is the ‘viscous” part of viscoelasticity. A number of experimental procedures are
available to probe and quantify the time dependence of this delayed response; this chapter will
consider just one of these: the creep test.
The creep test consists of measuring the time dependent strain (t) = δ(t)/L0 resulting from
the application of a steady uniaxial stress σ0 as illustrated in Fig. 2.13. These three curves are the
strains measured at three diﬀerent stress levels, each one twice the magnitude of the previous one.
Note in Fig. 2.13 that when the stress is doubled, the resulting strain in doubled over its full
range of time. This occurs if the materials is linear in its response. If the strain-stress relation is
2.3. VISCOELASTICITY 39
Figure 2.12: A generic modulus-temperature map for polymers.
Figure 2.13: Creep strain at various constant stresses.
linear, the strain resulting from a stress aσ, where a is a constant, is just the constant a times the
strain resulting from σ alone. Mathematically,
(aσ) = a (σ)
This is just a case of “double the stress, double the strain.”
If the creep strains produced at a given time are plotted as the abscissa against the applied stress
as the ordinate, an “isochronous” stress-strain curve would be produced. If the material is linear,
this “curve” will be a straight line, with a slope that increases as the chosen time is decreased.
For linear materials, the family of strain histories (t) obtained at various constant stresses may
be superimposed by normalizing them based on the applied stress. The ratio of strain to stress is
called the “compliance” C, and in the case of time-varying strain arising from a constant stress the
ratio is the “creep compliance”:
A typical form of this function is shown in Fig. 2.14, plotted against the logarithm of time. Note
that the logarithmic form of the plot changes the shape of the curve drastically, stretching out
the short-time portion of the response and compressing the long-time region. Upon loading, the
40 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
material strains initially to the “glassy” compliance Cg; this is the elastic deformation corresponding
to bond distortion. In time, the compliance rises exponentially to an equilibrium or “rubbery” value
Cr, corresponding to the rubbery extension of the material. The value along the abscissa labeled
“log τ” marks the inﬂection from rising to falling slope, and τ is called the “relaxation time” of the
Figure 2.14: The creep compliance function Ccrp(t).
By inspection, we can model the compliance function of Fig. 2.14 with a ﬁrst-order relation of
Ccrp(t) = Cg + (Cr − Cg) 1 − e
2.3.3 The Boltzman Superposition Integral
The stress-strain relations for viscoelastic materials can be written as either diﬀerential or integral
equations, and this section will explore the integral formulation.
Integrals are summing operations, and this view of viscoelasticity takes the response of the
material at time t to be the sum of the responses to excitations imposed at all previous times. The
ability to sum these individual responses requires the material to obey a more general statement of
linearity than we have invoked previously, speciﬁcally that the response to a number of individual
excitations be the sum of the responses that would have been generated by each excitation acting
alone. Mathematically, if the strain due to a stress σ1(t) is (σ1) and that due to a diﬀerent stress
σ2(t) is (σ2), then the strain due to both stresses is (σ1 + σ2) = (σ1) + (σ2). Combining this
with the condition for multiplicative scaling used earlier, we have as a general statement of linear
(aσ1 + bσ2) = a (σ1) + b (σ2) (2.18)
The “Boltzman Superposition Integral” statement of linear viscoelastic response follows from
this deﬁnition. Consider the strain 1(t) at time t due to the application of a small stress ∆σ1
applied at a time ξ1 previous to t; this is given directly from the deﬁnition of the creep compliance
1(t) = Ccrp(t − ξ1)∆σ1
Similarly, the strain 2(t) due to a stress increment ∆σ2 applied at a diﬀerent time ξ2 is
2.4. PROBLEMS 41
2(t) = Ccrp(t − ξ2)∆σ2
If the material is linear, the total strain at time t due to both strain increments together can be
obtained by superposition of these two individual eﬀects:
(t) = 1(t) + 2(t) = Ccrp(t − ξ1)∆σ1 + Ccrp(t − ξ2)∆σ2
As the number of applied strain increments increases so as to approach a continuous distribution,
Ccrp(t − ξj)∆σj
−→ (t) =
Ccrp(t − ξ) dσ =
Ccrp(t − ξ)
1. Aklonis, J.J., MacKnight, W.J., and Shen, M., Introduction to Polymer Viscoelasticity, Wiley-
Interscience, New York, 1972.
2. Callister, W.D., Materials Science and Engineering: An Introduction, J. Wiley, New York,
3. Williams, M.L., “Structural Analysis of Viscoelastic Materials,” AIAA Journal, p. 785, May
1. The Thermal Shock Resistance, or TSR, of an item relates to its resistance to fracture when
suddenly quenched from a high temperature to a lower one. Justify the expression for the
where k is the coeﬃcient of thermal conductivity. Look up reasonable values for these pa-
rameters, and compare the TSR of quartz, soda-lime and borosilicate (Pyrex) glass. Explain
the diﬀerences between these values on an atomistic basis.
2. A thin microelectronic “chip” is bonded to a much thicker substrate. Show that the biaxial
stress induced in the chip when the temperature is raised by ∆T is
σx = σy =
(αsubstrate − αchip) E ∆T
1 − ν
3. Show the stress-extension relationship for equi-biaxial extension (λx = λy ≡ λ to be
σtrue = 2NkT λ2
42 CHAPTER 2. THERMODYNAMICS OF MECHANICAL RESPONSE
4. Show the pressure-extension relationship for a spherical balloon to be
Plot the function on the right-hand-side, and explain why it shows a maximum (which is
readily felt when blowing up a party balloon).
5. Determine the apparent activation energy in (E† in Eqn. 2.16) for a viscoelastic relaxation in
which the initial rate is observed to double when the temperature is increased from 20◦C to
30◦C. (Answer: E† = 51 kJ/mol.)
6. Plot the strain response (t) to a load-unload stress input deﬁned as
0, t < 1
1, 1 < t < 4.5
−1, 4.5 < t < 5
0, t > 5
The material obeys the ﬁrst-order compliance law (Eqn. 2.17) with Cg = 5, Cr = 10, and
τ = 2.
This chapter introduces basic concepts of stiﬀness and strength underlying the mechanics of ﬁber-
reinforced advanced composite materials. This aspect of composite materials technology is some-
times terms “micromechanics,” because it deals with the relations between macroscopic engineering
properties and the microscopic distribution of the material’s constituents, namely the volume frac-
tion of ﬁber. This chapter will deal primarily with unidirectionally-reinforced continuous-ﬁber
composites, and with properties measured along and transverse to the ﬁber direction.
The term composite could mean almost anything if taken at face value, since all materials are
composed of dissimilar subunits if examined at close enough detail. But in modern materials engi-
neering, the term usually refers to a “matrix” material that is reinforced with ﬁbers. For instance,
the term “FRP” (for Fiber Reinforced Plastic) usually indicates a thermosetting polyester matrix
containing glass ﬁbers, and this particular composite has the lion’s share of today’s commercial
market. Figure 3.1 shows a laminate fabricated by “crossplying” unidirectionally-reinforced layers
in a 0◦-90◦stacking sequence.
Figure 3.1: A crossplied FRP laminate, showing nonuniform ﬁber packing and microcracking (from
44 CHAPTER 3. COMPOSITES
Many composites used today are at the leading edge of materials technology, with performance
and costs appropriate to ultrademanding applications such as spacecraft. But heterogeneous ma-
terials combining the best aspects of dissimilar constituents have been used by nature for millions
of years. Ancient society, imitating nature, used this approach as well: the Book of Exodus speaks
of using straw to reinforce mud in brickmaking, without which the bricks would have almost no
As seen in Table 3.11, the ﬁbers used in modern composites have strengths and stiﬀnesses
far above those of traditional bulk materials. The high strengths of the glass ﬁbers are due to
processing that avoids the internal or surface ﬂaws which normally weaken glass, and the strength
and stiﬀness of the polymeric aramid ﬁber is a consequence of the nearly perfect alignment of the
molecular chains with the ﬁber axis.
Table 3.1: Properties of Composite Reinforcing Fibers.
Material E σb b ρ E/ρ σb/ρ cost
(GPa) (GPa) (%) (Mg/m3
) (MJ/kg) (MJ/kg) ($/kg)
E-glass 72.4 2.4 2.6 2.54 28.5 0.95 1.1
S-glass 85.5 4.5 2.0 2.49 34.3 1.8 22–33
aramid 124 3.6 2.3 1.45 86 2.5 22–33
boron 400 3.5 1.0 2.45 163 1.43 330–440
HS graphite 253 4.5 1.1 1.80 140 2.5 66–110
HM graphite 520 2.4 0.6 1.85 281 1.3 220–660
Of course, these materials are not generally usable as ﬁbers alone, and typically they are im-
pregnated by a matrix material that acts to transfer loads to the ﬁbers, and also to protect the
ﬁbers from abrasion and environmental attack. The matrix dilutes the properties to some de-
gree, but even so very high speciﬁc (weight-adjusted) properties are available from these materials.
Metal and glass are available as matrix materials, but these are currently very expensive and
largely restricted to R&D laboratories. Polymers are much more commonly used, with unsatu-
rated styrene-hardened polyesters having the majority of low-to-medium performance applications
and epoxy or more sophisticated thermosets having the higher end of the market. Thermoplastic
matrix composites are increasingly attractive materials, with processing diﬃculties being perhaps
their principal limitation.
The ﬁbers may be oriented randomly within the material, but it is also possible to arrange for them
to be oriented preferentially in the direction expected to have the highest stresses. Such a material
is said to be anisotropic (diﬀerent properties in diﬀerent directions), and control of the anisotropy
is an important means of optimizing the material for speciﬁc applications. At a microscopic level,
the properties of these composites are determined by the orientation and distribution of the ﬁbers,
as well as by the properties of the ﬁber and matrix materials. The topic known as composite
micromechanics is concerned with developing estimates of the overall material properties from
F.P. Gerstle, “Composites,” Encyclopedia of Polymer Science and Engineering, Wiley, New York, 1991. Here E
is Young’s modulus, σb is breaking stress, b is breaking strain, and ρ is density.
3.2. STIFFNESS 45
Figure 3.2: Loading parallel to the ﬁbers.
Consider a typical region of material of unit dimensions, containing a volume fraction Vf of
ﬁbers all oriented in a single direction. The matrix volume fraction is then Vm = 1 − Vf . This
region can be idealized as shown in Fig. 3.2 by gathering all the ﬁbers together, leaving the matrix
to occupy the remaining volume — this is sometimes called the “slab model.” If a stress σ1 is
applied along the ﬁber direction, the ﬁber and matrix phases act in parallel to support the load. In
these parallel connections the strains in each phase must be the same, so the strain 1 in the ﬁber
direction can be written as:
f = m = 1
The forces in each phase must add to balance the total load on the material. Since the forces in
each phase are the phase stresses times the area (here numerically equal to the volume fraction),
σ1 = σf Vf + σmVm = Ef 1Vf + Em 1Vm
The stiﬀness in the ﬁber direction is found by dividing by the strain:
= Vf Ef + Vm Em (3.1)
This relation is known as a rule of mixtures prediction of the overall modulus in terms of the moduli
of the constituent phases and their volume fractions.
Figure 3.3: Loading perpendicular to the ﬁbers.
46 CHAPTER 3. COMPOSITES
If the stress is applied in the direction transverse to the ﬁbers as depicted in Fig. 3.3, the
slab model can be applied with the ﬁber and matrix materials acting in series. In this case the
stress in the ﬁber and matrix are equal (an idealization), but the deﬂections add to give the overall
transverse deﬂection. In this case it can be shown (see Prob. 1)
Figure 3.4 shows the functional form of the parallel (Eqn. 3.1) and series (Eqn. 3.2) predictions for
the ﬁber- and transverse-direction moduli.
Figure 3.4: Rule-of-mixtures predictions for longitudinal (E1) and transverse (E2) modulus, for
glass-polyester composite (Ef = 73.7 MPa, Em = 4 GPa). Experimental data taken from Hull
The prediction of transverse modulus given by the series slab model (Eqn. 3.2) is considered
unreliable, in spite of its occasional agreement with experiment. Among other deﬁciencies the
assumption of uniform matrix strain being untenable; both analytical and experimental studies
have shown substantial nonuniformity in the matrix strain. Figure 3.5 shows the photoelastic
fringes in the matrix caused by the perturbing eﬀect of the stiﬀer ﬁbers.
In more complicated composites, for instance those with ﬁbers in more than one direction or
those having particulate or other nonﬁbrous reinforcements, Eqn. 3.1 provides an upper bound to
the composite modulus, while Eqn. 3.2 is a lower bound (see Fig. 3.4). Most practical cases will be
somewhere between these two values, and the search for reasonable models for these intermediate
cases has occupied considerable attention in the composites research community. Perhaps the most
popular model is an empirical one known as the Halpin-Tsai equation2, which can be written in
Em[Ef + ξ(Vf Ef + VmEm)]
Vf Em + VmEf + ξEm
c.f. J.C.. Halpin and J.L. Kardos, Polymer Engineering and Science, Vol. 16, May 1976, pp. 344–352.
3.3. STRENGTH 47
Here ξ is an adjustable parameter that results in series coupling for ξ = 0 and parallel averaging
for very large ξ.
Figure 3.5: Photoelastic (isochromatic) fringes in a composite model subjected to transverse tension
(from Hull, 1996).
Rule of mixtures estimates for strength proceed along lines similar to those for stiﬀness. For
instance, consider a unidirectionally reinforced composite that is strained up to the value at which
the ﬁbers begin to break. Denoting this value fb, the stress transmitted by the composite is given
by multiplying the stiﬀness (Eqn. 3.1):
σb = fb E1 = Vf σfb + (1 − Vf )σ∗
The stress σ∗ is the stress in the matrix, which is given by fbEm. This relation is linear in Vf ,
rising from σ∗ to the ﬁber breaking strength σfb = Ef fb. However, this relation is not realistic at
low ﬁber concentration, since the breaking strain of the matrix mb is usually substantially greater
than fb. If the matrix had no ﬁbers in it, it would fail at a stress σmb = Em mb. If the ﬁbers were
considered to carry no load at all, having broken at = fb and leaving the matrix to carry the
remaining load, the strength of the composite would fall oﬀ with ﬁber fraction according to
σb = (1 − Vf )σmb
Since the breaking strength actually observed in the composite is the greater of these two expres-
sions, there will be a range of ﬁber fraction in which the composite is weakened by the addition of
ﬁbers. These relations are depicted in Fig. 3.6.
1. Ashton, J.E., J.C. Halpin and P.H. Petit, Primer on Composite Materials: Analysis,Technomic
Press, Westport, CT, 1969.